Engineering Materials 2An Introduction to Microstructures, Processing and Design
Engineering Materials 2An Introduction to Microstructures, Processing and DesignSecond EditionbyMichael F. AshbyandDavid R. H. JonesDepartment of Engineering, Cambridge University, EnglandOXFORD AUCKLAND BOSTON JOHANNESBURG MELBOURNE NEW DELHI
Contents General introduction ix A. Metals1. Metals 3 the generic metals and alloys; iron-based, copper-based, nickel-based, aluminium-based and titanium-based alloys; design data2. Metal structures 14 the range of metal structures that can be altered to get different properties: crystal and glass structure, structures of solutions and compounds, grain and phase boundaries, equilibrium shapes of grains and phases3. Equilibrium constitution and phase diagrams 25 how mixing elements to make an alloy can change their structure; examples: the lead–tin, copper–nickel and copper–zinc alloy systems4. Case studies in phase diagrams 34 choosing soft solders; pure silicon for microchips; making bubble-free ice5. The driving force for structural change 46 the work done during a structural change gives the driving force for the change; examples: solidiﬁcation, solid-state phase changes, precipitate coarsening, grain growth, recrystallisation; sizes of driving forces6. Kinetics of structural change: I – diffusive transformations 57 why transformation rates peak – the opposing claims of driving force and thermal activation; why latent heat and diffusion slow transformations down7. Kinetics of structural change: II – nucleation 68 how new phases nucleate in liquids and solids; why nucleation is helped by solid catalysts; examples: nucleation in plants, vapour trails, bubble chambers and caramel
vi Contents 8. Kinetics of structural change: III – displacive transformations 76 how we can avoid diffusive transformations by rapid cooling; the alternative – displacive (shear) transformations at the speed of sound 9. Case studies in phase transformations 89 artiﬁcial rain-making; ﬁne-grained castings; single crystals for semiconductors; amorphous metals10. The light alloys 100 where they score over steels; how they can be made stronger: solution, age and work hardening; thermal stability11. Steels: I – carbon steels 113 structures produced by diffusive changes; structures produced by displacive changes (martensite); why quenching and tempering can transform the strength of steels; the TTT diagram12. Steels: II – alloy steels 125 adding other elements gives hardenability (ease of martensite formation), solution strengthening, precipitation strengthening, corrosion resistance, and austenitic (f.c.c.) steels13. Case studies in steels 133 metallurgical detective work after a boiler explosion; welding steels together safely; the case of the broken hammer14. Production, forming and joining of metals 143 processing routes for metals; casting; plastic working; control of grain size; machining; joining; surface engineering B. Ceramics and glasses15. Ceramics and glasses 161 the generic ceramics and glasses: glasses, vitreous ceramics, high- technology ceramics, cements and concretes, natural ceramics (rocks and ice), ceramic composites; design data16. Structure of ceramics 167 crystalline ceramics; glassy ceramics; ceramic alloys; ceramic micro- structures: pure, vitreous and composite17. The mechanical properties of ceramics 177 high stiffness and hardness; poor toughness and thermal shock resistance; the excellent creep resistance of refractory ceramics
Contents vii18. The statistics of brittle fracture and case study 185 how the distribution of ﬂaw sizes gives a dispersion of strength: the Weibull distribution; why the strength falls with time (static fatigue); case study: the design of pressure windows19. Production, forming and joining of ceramics 194 processing routes for ceramics; making and pressing powders to shape; working glasses; making high-technology ceramics; joining ceramics; applications of high-performance ceramics20. Special topic: cements and concretes 207 historical background; cement chemistry; setting and hardening of cement; strength of cement and concrete; high-strength cements C. Polymers and composites21. Polymers 219 the generic polymers: thermoplastics, thermosets, elastomers, natural polymers; design data22. The structure of polymers 228 giant molecules and their architecture; molecular packing: amorphous or crystalline?23. Mechanical behaviour of polymers 238 how the modulus and strength depend on temperature and time24. Production, forming and joining of polymers 254 making giant molecules by polymerisation; polymer “alloys”; forming and joining polymers25. Composites: ﬁbrous, particulate and foamed 263 how adding ﬁbres or particles to polymers can improve their stiffness, strength and toughness; why foams are good for absorbing energy26. Special topic: wood 277 one of nature’s most successful composite materials D. Designing with metals, ceramics, polymers and composites27. Design with materials 289 the design-limiting properties of metals, ceramics, polymers and composites; design methodology
viii Contents28. Case studies in design 296 1. Designing with metals: conveyor drums for an iron ore terminal 296 2. Designing with ceramics: ice forces on offshore structures 303 3. Designing with polymers: a plastic wheel 308 4. Designing with composites: materials for violin bodies 312Appendix 1 Teaching yourself phase diagrams 320Appendix 2 Symbols and formulae 370Index 377
General introductionMaterials are evolving today faster than at any time in history. Industrial nationsregard the development of new and improved materials as an “underpinning tech-nology” – one which can stimulate innovation in all branches of engineering, makingpossible new designs for structures, appliances, engines, electrical and electronic de-vices, processing and energy conservation equipment, and much more. Many of thesenations have promoted government-backed initiatives to promote the developmentand exploitation of new materials: their lists generally include “high-performance”composites, new engineering ceramics, high-strength polymers, glassy metals, andnew high-temperature alloys for gas turbines. These initiatives are now being feltthroughout engineering, and have already stimulated design of a new and innovativerange of consumer products. So the engineer must be more aware of materials and their potential than everbefore. Innovation, often, takes the form of replacing a component made of one mater-ial (a metal, say) with one made of another (a polymer, perhaps), and then redesigningthe product to exploit, to the maximum, the potential offered by the change. Theengineer must compare and weigh the properties of competing materials with pre-cision: the balance, often, is a delicate one. It involves an understanding of the basicproperties of materials; of how these are controlled by processing; of how materialsare formed, joined and ﬁnished; and of the chain of reasoning that leads to a successfulchoice. This book aims to provide this understanding. It complements our other book onthe properties and applications of engineering materials,* but it is not necessary tohave read that to understand this. In it, we group materials into four classes: Metals,Ceramics, Polymers and Composites, and we examine each in turn. In any one classthere are common underlying structural features (the long-chain molecules in poly-mers, the intrinsic brittleness of ceramics, or the mixed materials of composites) which,ultimately, determine the strengths and weaknesses (the “design-limiting” properties)of each in the engineering context. And so, as you can see from the Contents list, the chapters are arranged in groups,with a group of chapters to describe each of the four classes of materials. In each groupwe ﬁrst introduce the major families of materials that go to make up each materialsclass. We then outline the main microstructural features of the class, and show howto process or treat them to get the structures (really, in the end, the properties) thatwe want. Each group of chapters is illustrated by Case Studies designed to help you* M. F. Ashby and D. R. H. Jones, Engineering Materials 1: An Introduction to their Properties and Applications,2nd edition, Butterworth-Heinemann, 1996.
x General introductionunderstand the basic material. And ﬁnally we look at the role of materials in thedesign of engineering devices, mechanisms or structures, and develop a methodologyfor materials selection. One subject – Phase Diagrams – can be heavy going. We havetried to overcome this by giving a short programmed-learning course on phase dia-grams. If you work through this when you come to the chapter on phase diagrams youwill know all you need to about the subject. It will take you about 4 hours. At the end of each chapter you will ﬁnd a set of problems: try to do them while thetopic is still fresh in your mind – in this way you will be able to consolidate, anddevelop, your ideas as you go along.To the lecturerThis book has been written as a second-level course for engineering students. It pro-vides a concise introduction to the microstructures and processing of materials (metals,ceramics, polymers and composites) and shows how these are related to the propertiesrequired in engineering design. It is designed to follow on from our ﬁrst-level text onthe properties and applications of engineering materials,* but it is completely self-contained and can be used by itself. Each chapter is designed to provide the content of a 50-minute lecture. Each blockof four or so chapters is backed up by a set of Case Studies, which illustrate and con-solidate the material they contain. There are special sections on design, and on suchmaterials as wood, cement and concrete. And there are problems for the student at theend of each chapter for which worked solutions can be obtained separately, from thepublisher. In order to ease the teaching of phase diagrams (often a difﬁcult topic forengineering students) we have included a programmed-learning text which has provedhelpful for our own students. We have tried to present the material in an uncomplicated way, and to make theexamples entertaining, while establishing basic physical concepts and their applicationto materials processing. We found that the best way to do this was to identify a smallset of “generic” materials of each class (of metals, of ceramics, etc.) which broadlytypiﬁed the class, and to base the development on these; they provide the pegs onwhich the discussion and examples are hung. But the lecturer who wishes to drawother materials into the discussion should not ﬁnd this difﬁcult.AcknowledgementsWe wish to thank Prof. G. A. Chadwick for permission to reprint Fig. A1.34 (p. 340)and K. J. Pascoe and Van Nostrand Reinhold Co. for permission to reprint Fig. A1.41(p. 344).* M. F. Ashby and D. R. H. Jones, Engineering Materials 1: An Introduction to their Properties and Applications,2nd edition, Butterworth-Heinemann, 1996.
Metals 3Chapter 1MetalsIntroductionThis ﬁrst group of chapters looks at metals. There are so many different metals– literally hundreds of them – that it is impossible to remember them all. It isn’tnecessary – nearly all have evolved from a few “generic” metals and are simply tuned-up modiﬁcations of the basic recipes. If you know about the generic metals, you knowmost of what you need. This chapter introduces the generic metals. But rather than bore you with a cata-logue we introduce them through three real engineering examples. They allow us notonly to ﬁnd examples of the uses of the main generic metals but also to introduce theall-important business of how the characteristics of each metal determine how it isused in practice.Metals for a model traction engineModel-making has become big business. The testing of scale models provides a cheapway of getting critical design information for things from Olympic yacht hulls to tidalbarrages. Architects sell their newest creations with the help of miniature versionscorrect to the nearest door-handle and garden shrub. And in an age of increasingleisure time, many people ﬁnd an outlet for their energies in making models – perhapsputting together a miniature aircraft from a kit of plastic parts or, at the other extreme,building a fully working model of a steam engine from the basic raw materials in theirown “garden-shed” machine shop. Figure 1.1 shows a model of a nineteenth-century steam traction engine built in ahome workshop from plans published in a well-known modellers’ magazine. Every-thing works just as it did in the original – the boiler even burns the same type of coalto raise steam – and the model is capable of towing an automobile! But what interestsus here is the large range of metals that were used in its construction, and the way inwhich their selection was dictated by the requirements of design. We begin by lookingat metals based on iron ( ferrous metals). Table 1.1 lists the generic iron-based metals. How are these metals used in the traction engine? The design loads in componentslike the wheels and frames are sufﬁciently low that mild steel, with a yield strength σyof around 220 MPa, is more than strong enough. It is also easy to cut, bend or machineto shape. And last, but not least, it is cheap.
4 Engineering Materials 2Fig. 1.1. A fully working model, one-sixth full size, of a steam traction engine of the type used on manyfarms a hundred years ago. The model can pull an automobile on a few litres of water and a handful of coal.But it is also a nice example of materials selection and design.Table 1.1 Generic iron-based metalsMetal Typical composition Typical uses (w t%)Low-carbon (“mild”) steel Fe + 0.04 to 0.3 C Low-stress uses. General constructional steel, suitable (+ ≈ 0.8 Mn) for welding.Medium-carbon steel Fe + 0.3 to 0.7 C Medium-stress uses: machinery parts – nuts andbolts, (+ ≈ 0.8 Mn) shafts, gears.High-carbon steel Fe + 0.7 to 1.7 C High-stress uses: springs, cutting tools, dies. (+ ≈ 0.8 Mn)Low-alloy steel Fe + 0.2 C 0.8 Mn High-stress uses: pressure vessels, aircraft parts. 1 Cr 2 NiHigh-alloy (“stainless”) Fe + 0.1 C 0.5 Mn High-temperature or anti-corrosion uses: chemical or steel 18 Cr 8 Ni steam plants.Cast iron Fe + 1.8 to 4 C Low-stress uses: cylinder blocks, drain pipes. (+ ≈ 0.8 Mn 2 Si)
Metals 5Fig. 1.2. A close-up of the mechanical lubricator on the traction engine. Unless the bore of the steamcylinder is kept oiled it will become worn and scored. The lubricator pumps small metered quantities ofsteam oil into the cylinder to stop this happening. The drive is taken from the piston rod by the ratchet andpawl arrangement. The stresses in the machinery – like the gear-wheel teeth or the drive shafts – are agood deal higher, and these parts are made from either medium-carbon, high-carbon orlow-alloy steels to give extra strength. However, there are a few components whereeven the strength of high-carbon steels as delivered “off the shelf” (σy ≈ 400 MPa)is not enough. We can see a good example in the mechanical lubricator, shown inFig. 1.2, which is essentially a high-pressure oil metering pump. This is driven by aratchet and pawl. These have sharp teeth which would quickly wear if they weremade of a soft alloy. But how do we raise the hardness above that of ordinary high-carbon steel? Well, medium- and high-carbon steels can be hardened to give a yieldstrength of up to 1000 MPa by heating them to bright red heat and then quenchingthem into cold water. Although the quench makes the hardened steel brittle, we canmake it tough again (though still hard) by tempering it – a process that involves heatingthe steel again, but to a much lower temperature. And so the ratchet and pawls aremade from a quenched and tempered high-carbon steel. Stainless steel is used in several places. Figure 1.3 shows the ﬁre grate – the metalbars which carry the burning coals inside the ﬁrebox. When the engine is workinghard the coal is white hot; then, both oxidation and creep are problems. Mild steel barscan burn out in a season, but stainless steel bars last indeﬁnitely.
6 Engineering Materials 2Fig. 1.3. The ﬁre grate, which carries the white-hot ﬁre inside the ﬁrebox, must resist oxidation and creep.Stainless steel is best for this application. Note also the threaded monel stays which hold the ﬁrebox sidestogether against the internal pressure of the steam. Finally, what about cast iron? Although this is rather brittle, it is ﬁne for low-stressedcomponents like the cylinder block. In fact, because cast iron has a lot of carbon it hasseveral advantages over mild steel. Complicated components like the cylinder blockare best produced by casting. Now cast iron melts much more easily than steel (addingcarbon reduces the melting point in just the way that adding anti-freeze works withwater) and this makes the pouring of the castings much easier. During casting, thecarbon can be made to separate out as tiny particles of graphite, distributed through-out the iron, which make an ideal boundary lubricant. Cylinders and pistons madefrom cast iron wear very well; look inside the cylinders of your car engine next timethe head has to come off, and you will be amazed by the polished, almost glazed lookof the bores – and this after perhaps 108 piston strokes. These, then, are the basic classes of ferrous alloys. Their compositions and uses aresummarised in Table 1.1, and you will learn more about them in Chapters 11 and 12,but let us now look at the other generic alloy groups. An important group of alloys are those based on copper (Table 1.2). The most notable part of the traction engine made from copper is the boiler and itsﬁretubes (see Fig. 1.1). In full size this would have been made from mild steel, and theuse of copper in the model is a nice example of how the choice of material can dependon the scale of the structure. The boiler plates of the full-size engine are about 10 mmthick, of which perhaps only 6 mm is needed to stand the load from the pressurised
Metals 7Table 1.2 Generic copper-based metalsMetal Typical composition (w t%) Typical usesCopper 100 Cu Ductile, corrosion resistant and a good electrical conductor: water pipes, electrical wiring.Brass Zn Stronger than copper, machinable, reasonable corrosion resistance: water ﬁttings, screws, electrical components.Bronze Cu + 10–30 Sn Good corrosion resistance: bearings, ships’ propellers, bells.Cupronickel Cu + 30 Ni Good corrosion resistance, coinage.steam safely – the other 4 mm is an allowance for corrosion. Although a model steelboiler would stand the pressure with plates only 1 mm thick, it would still need thesame corrosion allowance of 4 mm, totalling 5 mm altogether. This would mean a veryheavy boiler, and a lot of water space would be taken up by thick plates and ﬁretubes.Because copper hardly corrodes in clean water, this is the obvious material to use.Although weaker than steel, copper plates 2.5 mm thick are strong enough to resist theworking pressure, and there is no need for a separate corrosion allowance. Of course,copper is expensive – it would be prohibitive in full size – but this is balanced by itsductility (it is very easy to bend and ﬂange to shape) and by its high thermal conduct-ivity (which means that the boiler steams very freely). Brass is stronger than copper, is much easier to machine, and is fairly corrosion-proof (although it can “dezincify” in water after a long time). A good example of itsuse in the engine is for steam valves and other boiler ﬁttings (see Fig. 1.4). These areintricate, and must be easy to machine; dezinciﬁcation is a long-term possibility, sooccasional inspection is needed. Alternatively, corrosion can be avoided altogether byusing the more expensive bronzes, although some are hard to machine. Nickel and its alloys form another important class of non-ferrous metals (Table 1.3).The superb creep resistance of the nickel-based superalloys is a key factor in designingthe modern gas-turbine aero-engine. But nickel alloys even appear in a model steamengine. The ﬂat plates in the ﬁrebox must be stayed together to resist the internalsteam pressure (see Fig. 1.3). Some model-builders make these stays from pieces ofmonel rod because it is much stronger than copper, takes threads much better and isvery corrosion resistant.Metals for drinks cansFew people would think that the humble drink can (Fig. 1.5) was anything special. Butto a materials engineer it is high technology. Look at the requirements. As far aspossible we want to avoid seams. The can must not leak, should use as little metal aspossible and be recyclable. We have to choose a metal that is ductile to the point thatit can be drawn into a single-piece can body from one small slug of metal. It must notcorrode in beer or coke and, of course, it must be non-toxic. And it must be light andmust cost almost nothing.
8 Engineering Materials 2Fig. 1.4. Miniature boiler ﬁttings made from brass: a water-level gauge, a steam valve, a pressure gauge,and a feed-water injector. Brass is so easy to machine that it is good for intricate parts like these.Table 1.3 Generic nickel-based metalsMetals Typical composition (w t%) Typical usesMonels Ni + 30 Cu 1 Fe 1 Mn Strong, corrosion resistant: heat-exchanger tubes.Superalloys Ni + 30 Cr 30 Fe 0.5 Ti 0.5 Al Creep and oxidation resistant: furnace parts. Ni + 10 Co 10 W 9 Cr 5 A12 Ti Highly creep resistant: turbine blades and discs. Aluminium-based metals are the obvious choice* (Table 1.4) – they are light, corro-sion resistant and non-toxic. But it took several years to develop the process for form-ing the can and the alloy to go with it. The end product is a big advance from the dayswhen drinks only came in glass bottles, and has created a new market for aluminium(now threatened, as we shall see in Chapter 21, by polymers). Because aluminium is* One thinks of aluminium as a cheap material – aluminium spoons are so cheap that they are thrown away.It was not always so. Napoleon had a set of cutlery specially made from the then-new material. It cost himmore than a set of solid silver.
Metals 9Fig. 1.5. The aluminium drink can is an innovative product. The body is made from a single slug of a3000 series aluminium alloy. The can top is a separate pressing which is fastened to the body by a rolledseam once the can has been ﬁlled. There are limits to one-piece construction.Table 1.4 Generic aluminium-based metalsMetal Typical composition (w t%) Typical uses1000 Series > 99 Al Weak but ductile and a good electrical unalloyed Al conductor: power transmission lines, cooking foil.2000 Series Al + 4 Cu + Mg, Si, Mn Strong age-hardening alloy: aircraft skins, spars, major additive Cu forgings, rivets.3000 Series Al + 1 Mn Moderate strength, ductile, excellent corrosion resistance: major additive Mn rooﬁng sheet, cooking pans, drinks can bodies.5000 Series Al + 3 Mg 0.5 Mn Strong work-hardening weldable plate: pressure major additive Mg vessels, ship superstructures.6000 Series Al + 0.5 Mg 0.5 Si Moderate-strength age-hardening alloy: anodised major additives extruded sections, e.g. window frames. Mg + Si7000 Series Al + 6 Zn + Mg, Cu, Mn Strong age-hardening alloy: aircraft forgings, major additives sparts, lightweight railway carriage shells. Zn + MgCasting alloys Al + 11 Si Sand and die castings.Aluminium– Al + 3 Li Low density and good strength: aircraft skins lithium alloys and spars.
10 Engineering Materials 2lighter than most other metals it is also the obvious choice for transportation: aircraft,high-speed trains, cars, even. Most of the alloys listed in Table 1.4 are designed withthese uses in mind. We will discuss the origin of their strength, and their uses, in moredetail in Chapter 10.Metals for artiﬁcial hip jointsAs a last example we turn to the world of medicine. Osteo-arthritis is an illness thataffects many people as they get older. The disease affects the joints between differentbones in the body and makes it hard – and painful – to move them. The problem iscaused by small lumps of bone which grow on the rubbing surfaces of the joints andwhich prevent them sliding properly. The problem can only be cured by removing thebad joints and putting artiﬁcial joints in their place. The ﬁrst recorded hip-joint re-placement was done as far back as 1897 – when it must have been a pretty hazardousbusiness – but the operation is now a routine piece of orthopaedic surgery. In fact30,000 hip joints are replaced in the UK every year; world-wide the number mustapproach half a million. Figure 1.6 shows the implant for a replacement hip joint. In the operation, the headof the femur is cut off and the soft marrow is taken out to make a hole down the centreof the bone. Into the hole is glued a long metal shank which carries the artiﬁcial head.Fig. 1.6. The titanium alloy implant for a replacement hip joint. The long shank is glued into the top of thefemur. The spherical head engages in a high-density polythene socket which is glued into the pelvic socket.
Metals 11Table 1.5 Generic titanium-based metalsMetal Typical composition (w t%) Typical usesa–b titanium alloy Ti–6 A14 V Light, very strong, excellent corrosion resistance, high melting point, good creep resistance. The alloy workhorse: turbofans, airframes, chemical plant, surgical implants.This ﬁts into a high-density polythene socket which in turn is glued into the old bonesocket. The requirements of the implant are stringent. It has to take large loads with-out bending. Every time the joint is used (≈106 times a year) the load on it ﬂuctuates,giving us a high-cycle fatigue problem as well. Body ﬂuids are as corrosive as seawater, so we must design against corrosion, stress corrosion and corrosion fatigue. Themetal must be bio-compatible. And, ideally, it should be light as well. The materials that best meet these tough requirements are based on titanium. Theα–β alloy shown in Table 1.5 is as strong as a hardened and tempered high-carbonsteel, is more corrosion resistant in body ﬂuids than stainless steel, but is only halfthe weight. A disadvantage is that its modulus is only half that of steels, so that ittends to be “whippy” under load. But this can be overcome by using slightly stiffersections. The same alloy is used in aircraft, both in the airframes and in the compressorstages of the gas turbines which drive them.Data for metalsWhen you select a metal for any design application you need data for the properties.Table 1.6 gives you approximate property data for the main generic metals, useful forthe ﬁrst phase of a design project. When you have narrowed down your choice youshould turn to the more exhaustive data compilations given under Further Reading.Finally, before making ﬁnal design decisions you should get detailed material speciﬁca-tions from the supplier who will provide the materials you intend to use. And if thecomponent is a critical one (meaning that its failure could precipitate a catastrophe)you should arrange to test it yourself. There are, of course, many more metals available than those listed here. It is use-ful to know that some properties depend very little on microstructure: the density,modulus, thermal expansion and speciﬁc heat of any steel are pretty close to those listedin the table. (Look at the table and you will see that the variations in these properties areseldom more than ±5%.) These are the “structure-insensitive” properties. Other proper-ties, though, vary greatly with the heat treatment and mechanical treatment, and thedetailed alloy composition. These are the “structure-sensitive” properties: yield andtensile strength, ductility, fracture toughness, and creep and fatigue strength. Theycannot be guessed from data for other alloys, even when the composition is almost thesame. For these it is essential to consult manufacturers’ data sheets listing the proper-ties of the alloy you intend to use, with the same mechanical and heat treatment.
Metals 13Ductility Fracture Melting Speciﬁc Thermal Thermal toughness temperature heat conductivity expansion (MPa m1/2) (K) (J kg −1 K −1) (W m −1 K −1) coefﬁcient (MK −1) 0.3 80 1809 456 78 12 0.21 140 1765 482 60 12 0.1–0.2 20–50 1570 460 40 12 0.1–0.2 50–170 1750 460 40 12 0.1–0.5 50–170 1680 500 12–30 10–18 0–0.18 6–20 1403 0.5–0.9 >100 1356 385 397 17 0.5 30–100 1190 121 20 0.5 30–100 1120 85 19 0.4 >100 1728 450 89 13 0.5 >100 1600 420 22 14 0.2 >100 1550 450 11 12 0.1–0.5 45 933 917 240 24 0.1–0.45 45 915 24 0.1–0.25 10–50 860 180 24 0.1–0.35 30–40 890 130 22 0.1–0.17 20–70 890 150 240.01–0.15 5–30 860 140 20 0.25 1940 530 22 9 0.1–0.2 50–80 1920 610 6 8 0.4 693 390 120 31 4560.07–0.15 650 420 110 27 wear resistance, thermal conductivity, electrical conductivity. Structure-insensitive properties: elastic moduli, Poisson’s ratio, density, thermal expansion coefﬁcient, speciﬁc heat.1.2 What are the ﬁve main generic classes of metals? For each generic class:(a) give one example of a speciﬁc component made from that class;(b) indicate why that class was selected for the component.
14 Engineering Materials 2Chapter 2Metal structuresIntroductionAt the end of Chapter 1 we noted that structure-sensitive properties like strength,ductility or toughness depend critically on things like the composition of the metaland on whether it has been heated, quenched or cold formed. Alloying or heat treatingwork by controlling the structure of the metal. Table 2.1 shows the large range overwhich a material has structure. The bracketed subset in the table can be controlled togive a wide choice of structure-sensitive properties.Table 2.1Structural feature Typical scale (m)Nuclear structure 10 −15Structure of atom 10 −10Crystal or glass structure 10 −9 5Structures of solutions and compounds 10 −9 4Structures of grain and phase boundaries 10 −8 6 Range that can be controlled to alter propertiesShapes of grains and phases 10 −7 to 10 −3 4Aggregates of grains 10 −5 to 10 −2 7Engineering structures 10 −3 to 10 3Crystal and glass structuresWe begin by looking at the smallest scale of controllable structural feature – the way inwhich the atoms in the metals are packed together to give either a crystalline or aglassy (amorphous) structure. Table 2.2 lists the crystal structures of the pure metals atroom temperature. In nearly every case the metal atoms pack into the simple crystalstructures of face-centred cubic (f.c.c.), body-centred cubic (b.c.c.) or close-packedhexagonal (c.p.h.). Metal atoms tend to behave like miniature ball-bearings and tend to pack togetheras tightly as possible. F.c.c. and c.p.h. give the highest possible packing density, with74% of the volume of the metal taken up by the atomic spheres. However, in somemetals, like iron or chromium, the metallic bond has some directionality and this makesthe atoms pack into the more open b.c.c. structure with a packing density of 68%. Some metals have more than one crystal structure. The most important examples areiron and titanium. As Fig. 2.1 shows, iron changes from b.c.c. to f.c.c. at 914°C but goes
Metal structures 15 Table 2.2 Crystal structures of pure metals at room temperature Pure metal Structure Unit cell dimensions (nm) a c Aluminium f.c.c. 0.405 Beryllium c.p.h. 0.229 0.358 Cadmium c.p.h. 0.298 0.562 Chromium b.c.c. 0.289 Cobalt c.p.h. 0.251 0.409 Copper f.c.c. 0.362 Gold f.c.c. 0.408 Hafnium c.p.h. 0.320 0.506 Indium Face-centred tetragonal Iridium f.c.c. 0.384 Iron b.c.c. 0.287 Lanthanum c.p.h. 0.376 0.606 Lead f.c.c. 0.495 Magnesium c.p.h. 0.321 0.521 Manganese Cubic 0.891 Molybdenum b.c.c. 0.315 Nickel f.c.c. 0.352 Niobium b.c.c. 0.330 Palladium f.c.c. 0.389 Platinum f.c.c. 0.392 Rhodium f.c.c. 0.380 Silver f.c.c. 0.409 Tantalum b.c.c. 0.331 Thallium c.p.h. 0.346 0.553 Tin Body-centred tetragonal Titanium c.p.h. 0.295 0.468 Tungsten b.c.c. 0.317 Vanadium b.c.c. 0.303 Yttrium c.p.h. 0.365 0.573 Zinc c.p.h. 0.267 0.495 Zirconium c.p.h. 0.323 0.515Fig. 2.1. Some metals have more than one crystal structure. The most important examples of thispolymorphism are in iron and titanium.
16 Engineering Materials 2back to b.c.c. at 1391°C; and titanium changes from c.p.h. to b.c.c. at 882°C. Thismultiplicity of crystal structures is called polymorphism. But it is obviously out of thequestion to try to control crystal structure simply by changing the temperature (iron isuseless as a structural material well below 914°C). Polymorphism can, however, bebrought about at room temperature by alloying. Indeed, many stainless steels are f.c.c.rather than b.c.c. and, especially at low temperatures, have much better ductility andtoughness than ordinary carbon steels. This is why stainless steel is so good for cryogenic work: the fast fracture of a steelvacuum ﬂask containing liquid nitrogen would be embarrassing, to say the least, butstainless steel is essential for the vacuum jackets needed to cool the latest supercon-ducting magnets down to liquid helium temperatures, or for storing liquid hydrogenor oxygen. If molten metals (or, more usually, alloys) are cooled very fast – faster than about106 K s−1 – there is no time for the randomly arranged atoms in the liquid to switch intothe orderly arrangement of a solid crystal. Instead, a glassy or amorphous solid is pro-duced which has essentially a “frozen-in” liquid structure. This structure – which istermed dense random packing (drp) – can be modelled very well by pouring ball-bearingsinto a glass jar and shaking them down to maximise the packing density. It is interest-ing to see that, although this structure is disordered, it has well-deﬁned characteristics.For example, the packing density is always 64%, which is why corn was always sold inbushels (1 bushel = 8 UK gallons): provided the corn was always shaken down well inthe sack a bushel always gave 0.64 × 8 = 5.12 gallons of corn material! It has onlyrecently become practicable to make glassy metals in quantity but, because their struc-ture is so different from that of “normal” metals, they have some very unusual andexciting properties.Structures of solutions and compoundsAs you can see from the tables in Chapter 1, few metals are used in their pure state –they nearly always have other elements added to them which turn them into alloys andgive them better mechanical properties. The alloying elements will always dissolve inthe basic metal to form solid solutions, although the solubility can vary between <0.01%and 100% depending on the combinations of elements we choose. As examples, theiron in a carbon steel can only dissolve 0.007% carbon at room temperature; the copperin brass can dissolve more than 30% zinc; and the copper–nickel system – the basis ofthe monels and the cupronickels – has complete solid solubility. There are two basic classes of solid solution. In the ﬁrst, small atoms (like carbon,boron and most gases) ﬁt between the larger metal atoms to give interstitial solidsolutions (Fig. 2.2a). Although this interstitial solubility is usually limited to a few percent it can have a large effect on properties. Indeed, as we shall see later, interstitialsolutions of carbon in iron are largely responsible for the enormous range of strengthsthat we can get from carbon steels. It is much more common, though, for the dissolvedatoms to have a similar size to those of the host metal. Then the dissolved atoms
Metal structures 17Fig. 2.2. Solid-solution structures. In interstitial solutions small atoms ﬁt into the spaces between large atoms.In substitutional solutions similarly sized atoms replace one another. If A–A, A–B and B–B bonds have thesame strength then this replacement is random. But unequal bond strengths can give clustering or ordering.simply replace some of the host atoms to give a substitutional solid solution (Fig. 2.2b).Brass and cupronickel are good examples of the large solubilities that this atomicsubstitution can give. Solutions normally tend to be random so that one cannot predict which of the siteswill be occupied by which atoms (Fig. 2.2c). But if A atoms prefer to have A neigh-bours, or B atoms prefer B neighbours, the solution can cluster (Fig. 2.2d); and when Aatoms prefer B neighbours the solution can order (Fig. 2.2e). Many alloys contain more of the alloying elements than the host metal can dissolve.Then the surplus must separate out to give regions that have a high concentration ofthe alloying element. In a few alloys these regions consist of a solid solution based onthe alloying element. (The lead–tin alloy system, on which most soft solders are based,Table 1.6, is a nice example of this – the lead can only dissolve 2% tin at room temper-ature and any surplus tin will separate out as regions of tin containing 0.3% dissolvedlead.) In most alloy systems, however, the surplus atoms of the alloying elementseparate out as chemical compounds. An important example of this is in the aluminium–copper system (the basis of the 2000 series alloys, Table 1.4) where surplus copperseparates out as the compound CuAl2. CuAl2 is hard and is not easily cut by disloca-tions. And when it is ﬁnely dispersed throughout the alloy it can give very bigincreases in strength. Other important compounds are Ni3Al, Ni3Ti, Mo2C and TaC (insuper-alloys) and Fe3C (in carbon steels). Figure 2.3 shows the crystal structure ofCuAl2. As with most compounds, it is quite complicated.
18 Engineering Materials 2Fig. 2.3. The crystal structure of the “intermetallic” compound CuAl2. The structures of compounds are usuallymore complicated than those of pure metals.PhasesThe things that we have been talking about so far – metal crystals, amorphous metals,solid solutions, and solid compounds – are all phases. A phase is a region of materialthat has uniform physical and chemical properties. Water is a phase – any one drop ofwater is the same as the next. Ice is another phase – one splinter of ice is the same asany other. But the mixture of ice and water in your glass at dinner is not a single phasebecause its properties vary as you move from water to ice. Ice + water is a two-phasemixture.Grain and phase boundariesA pure metal, or a solid solution, is single-phase. It is certainly possible to make singlecrystals of metals or alloys but it is difﬁcult and the expense is only worth it for high-technology applications such as single-crystal turbine blades or single-crystal siliconfor microchips. Normally, any single-phase metal is polycrystalline – it is made up ofmillions of small crystals, or grains, “stuck” together by grain boundaries (Fig. 2.4).Fig. 2.4. The structure of a typical grain boundary. In order to “bridge the gap” between two crystals ofdifferent orientation the atoms in the grain boundary have to be packed in a less ordered way. The packingdensity in the boundary is then as low as 50%.
Metal structures 19Fig. 2.5. Structures of interphase boundaries.Because of their unusual structure, grain boundaries have special properties of theirown. First, the lower bond density in the boundary is associated with a boundarysurface-energy: typically 0.5 Joules per square metre of boundary area (0.5 J m−2).Secondly, the more open structure of the boundary can give much faster diffusion inthe boundary plane than in the crystal on either side. And ﬁnally, the extra spacemakes it easier for outsized impurity atoms to dissolve in the boundary. These atomstend to segregate to the boundaries, sometimes very strongly. Then an average impurityconcentration of a few parts per million can give a local concentration of 10% in theboundary with very damaging effects on the fracture toughness.* As we have already seen, when an alloy contains more of the alloying element thanthe host metal can dissolve, it will split up into two phases. The two phases are “stuck”together by interphase boundaries which, again, have special properties of their own. Welook ﬁrst at two phases which have different chemical compositions but the samecrystal structure (Fig. 2.5a). Provided they are oriented in the right way, the crystalscan be made to match up at the boundary. Then, although there is a sharp change in* Henry Bessemer, the great Victorian ironmaster and the ﬁrst person to mass-produce mild steel, wasnearly bankrupted by this. When he changed his suppliers of iron ore, his steel began to crack in service.The new ore contained phosphorus, which we now know segregates badly to grain boundaries. Modernsteels must contain less than ≈0.05% phosphorus as a result.
20 Engineering Materials 2chemical composition, there is no structural change, and the energy of this coherentboundary is low (typically 0.05 J m−2). If the two crystals have slightly different latticespacings, the boundary is still coherent but has some strain (and more energy) associ-ated with it (Fig. 2.5b). The strain obviously gets bigger as the boundary grows side-ways: full coherency is usually possible only with small second-phase particles. As theparticle grows, the strain builds up until it is relieved by the injection of dislocations togive a semi-coherent boundary (Fig. 2.5c). Often the two phases which meet at theboundary are large, and differ in both chemical composition and crystal structure.Then the boundary between them is incoherent; it is like a grain boundary across whichthere is also a change in chemical composition (Fig. 2.5d). Such a phase boundary hasa high energy – comparable with that of a grain boundary – and around 0.5 J m−2.Shapes of grains and phasesGrains come in all shapes and sizes, and both shape and size can have a big effect onthe properties of the polycrystalline metal (a good example is mild steel – its strengthcan be doubled by a ten-times decrease in grain size). Grain shape is strongly affectedby the way in which the metal is processed. Rolling or forging, for instance, can givestretched-out (or “textured”) grains; and in casting the solidifying grains are oftenelongated in the direction of the easiest heat loss. But if there are no external effectslike these, then the energy of the grain boundaries is the important thing. This can beillustrated very nicely by looking at a “two-dimensional” array of soap bubbles in athin glass cell. The soap ﬁlm minimises its overall energy by straightening out; and atthe corners of the bubbles the ﬁlms meet at angles of 120° to balance the surfacetensions (Fig. 2.6a). Of course a polycrystalline metal is three-dimensional, but thesame principles apply: the grain boundaries try to form themselves into ﬂat planes,and these planes always try to meet at 120°. A grain shape does indeed exist which notonly satisﬁes these conditions but also packs together to ﬁll space. It has 14 faces, andis therefore called a tetrakaidecahedron (Fig. 2.6b). This shape is remarkable, not onlyfor the properties just given, but because it appears in almost every physical science(the shape of cells in plants, of bubbles in foams, of grains in metals and of Dirichletcells in solid-state physics).* If the metal consists of two phases then we can get more shapes. The simplest iswhen a single-crystal particle of one phase forms inside a grain of another phase.Then, if the energy of the interphase boundary is isotropic (the same for all orientations),the second-phase particle will try to be spherical in order to minimise the interphaseboundary energy (Fig. 2.7a). Naturally, if coherency is possible along some planes, butnot along others, the particle will tend to grow as a plate, extensive along the low-energy planes but narrow along the high-energy ones (Fig. 2.7b). Phase shapes get morecomplicated when interphase boundaries and grain boundaries meet. Figure 2.7(c)shows the shape of a second-phase particle that has formed at a grain boundary. Theparticle is shaped by two spherical caps which meet the grain boundary at an angle θ.This angle is set by the balance of boundary tensions* For a long time it was thought that soap foams, grains in metals and so on were icosahedra. It took LordKelvin (of the degree K) to get it right.
Metal structures 21Fig. 2.6. (a) The surface energy of a “two-dimensional” array of soap bubbles is minimised if the soap ﬁlmsstraighten out. Where ﬁlms meet the forces of surface tension must balance. This can only happen if ﬁlms meetin “120° three-somes”.Fig. 2.6. (b) In a three-dimensional polycrystal the grain boundary energy is minimised if the boundariesﬂatten out. These ﬂats must meet in 120° three-somes to balance the grain boundary tensions. If we ﬁll spacewith equally sized tetrakaidecahedra we will satisfy these conditions. Grains in polycrystals therefore tend tobe shaped like tetrakaidecahedra when the grain-boundary energy is the dominating inﬂuence.
22 Engineering Materials 2Fig. 2.7. Many metals are made up of two phases. This ﬁgure shows some of the shapes that they canhave when boundary energies dominate. To keep things simple we have sectioned the tetrakaidecahedralgrains in the way that we did in Fig. 2.6(b). Note that Greek letters are often used to indicate phases. Wehave called the major phase a and the second phase b. But g is the symbol for the energy (or tension) ofgrain boundaries (ggb) and interphase interfaces (gab ). 2γαβ cos θ = γgb (2.1)where γαβ is the tension (or energy) of the interphase boundary and γgb is the grainboundary tension (or energy). In some alloys, γαβ can be թ γgb /2 in which case θ = 0. The second phase will thenspread along the boundary as a thin layer of β. This “wetting” of the grain boundarycan be a great nuisance – if the phase is brittle then cracks can spread along the grainboundaries until the metal falls apart completely. A favourite scientiﬁc party trick is toput some aluminium sheet in a dish of molten gallium and watch the individual grainsof aluminium come apart as the gallium whizzes down the boundary. The second phase can, of course, form complete grains (Fig. 2.7d). But only if γαβand γgb are similar will the phases have tetrakaidecahedral shapes where they cometogether. In general, γαβ and γgb may be quite different and the grains then have morecomplicated shapes.Summary: constitution and structureThe structure of a metal is deﬁned by two things. The ﬁrst is the constitution:(a) The overall composition – the elements (or components) that the metal contains and the relative weights of each of them.
Metal structures 23(b) The number of phases, and their relative weights.(c) The composition of each phase.The second is the geometric information about shape and size:(d) The shape of each phase.(e) The sizes and spacings of the phases.Armed with this information, we are in a strong position to re-examine the mechan-ical properties, and explain the great differences in strength, or toughness, or cor-rosion resistance between alloys. But where does this information come from? Theconstitution of an alloy is summarised by its phase diagram – the subject of the nextchapter. The shape and size are more difﬁcult, since they depend on the details of howthe alloy was made. But, as we shall see from later chapters, a fascinating range ofmicroscopic processes operates when metals are cast, or worked or heat-treated intoﬁnished products; and by understanding these, shape and size can, to a large extent,be predicted.Background readingM. F. Ashby and D. R. H. Jones, Engineering Materials I, 2nd edition, Butterworth-Heinemann, 1996.Further readingD. A. Porter and K. E. Easterling, Phase Transformations in Metals and Alloys, 2nd edition, Chapman and Hall, 1992.G. A. Chadwick, Metallography of Phase Transformations, Butterworth, 1972.Problems2.1 Describe, in a few words, with an example or sketch where appropriate, what is meant by each of the following: (a) polymorphism; (b) dense random packing; (c) an interstitial solid solution; (d) a substitutional solid solution; (e) clustering in solid solutions; (f ) ordering in solid solutions; (g) an intermetallic compound; (h) a phase in a metal; (i) a grain boundary; (j) an interphase boundary;
24 Engineering Materials 2 (k) a coherent interphase boundary; (l) a semi-coherent interphase boundary; (m) an incoherent interphase boundary; (n) the constitution of a metal; (o) a component in a metal.
Equilibrium constitution and phase diagrams 25Chapter 3Equilibrium constitution and phase diagramsIntroductionWhenever you have to report on the structure of an alloy – because it is a possibledesign choice, or because it has mysteriously failed in service – the ﬁrst thing youshould do is reach for its phase diagram. It tells you what, at equilibrium, the constitu-tion of the alloy should be. The real constitution may not be the equilibrium one, butthe equilibrium constitution gives a base line from which other non-equilibrium con-stitutions can be inferred. Using phase diagrams is like reading a map. We can explain how they work, butyou will not feel conﬁdent until you have used them. Hands-on experience is essential.So, although this chapter introduces you to phase diagrams, it is important for you towork through the “Teaching Yourself Phase Diagrams” section at the end of the book.This includes many short examples which give you direct experience of using thediagrams. The whole thing will only take you about four hours and we have tried tomake it interesting, even entertaining. But ﬁrst, a reminder of some essential deﬁnitions.DeﬁnitionsAn alloy is a metal made by taking a pure metal and adding other elements (the“alloying elements”) to it. Examples are brass (Cu + Zn) and monel (Ni + Cu). The components of an alloy are the elements which make it up. In brass, the compon-ents are copper and zinc. In monel they are nickel and copper. The components aregiven the atomic symbols, e.g. Cu, Zn or Ni, Cu. An alloy system is all the alloys you can make with a given set of components: “theCu–Zn system” describes all the alloys you can make from copper and zinc. A binaryalloy has two components; a ternary alloy has three. A phase is a region of material that has uniform physical and chemical properties.Phases are often given Greek symbols, like α or β. But when a phase consists of a solidsolution of an alloying element in a host metal, a clearer symbol can be used. As anexample, the phases in the lead–tin system may be symbolised as (Pb) – for the solu-tion of tin in lead, and (Sn) – for the solution of lead in tin. The composition of an alloy, or of a phase in an alloy, is usually measured in weight%, and is given the symbol W. Thus, in an imaginary A–B alloy system: wt of A WA = × 100%, (3.1) wt of A + wt of B wt of B WB = × 100%, (3.2) wt of A + wt of B
26 Engineering Materials 2and WA + WB = 100%. (3.3)Sometimes it is helpful to deﬁne the atom (or mol)%, given by atoms of A XA = × 100% (3.4) atoms of A + atoms of Band so on. The constitution of an alloy is described by(a) the overall composition;(b) the number of phases;(c) the composition of each phase;(d) the proportion by weight of each phase.An alloy has its equilibrium constitution when there is no further tendency for theconstitution to change with time. The equilibrium diagram or phase diagram summarises the equilibrium constitutionof the alloy system.The lead–tin phase diagramAnd now for a real phase diagram. We have chosen the lead–tin diagram (Fig. 3.1) asour example because it is pretty straightforward and we already know a bit about it.Indeed, if you have soldered electronic components together or used soldered pipeﬁttings in your hot-water layout, you will already have had some direct experience ofthis system.Fig. 3.1. The phase diagram for the lead–tin alloy system. There are three phases: L – a liquid solution oflead and tin; (Pb) – a solid solution of tin in lead; and (Sn) – a solid solution of lead in tin. The diagram isdivided up into six ﬁelds – three of them are single-phase, and three are two-phase.
Equilibrium constitution and phase diagrams 27 As in all binary phase diagrams, we have plotted the composition of the alloy on thehorizontal scale (in weight %), and the temperature on the vertical scale. The diagramis simply a two-dimensional map (drawn up from experimental data on the lead–tinsystem) which shows us where the various phases are in composition–temperaturespace. But how do we use the diagram in practice? As a ﬁrst example, take an alloy ofoverall composition 50 wt% lead at 170°C. The constitution point (Fig. 3.2a) lies inside atwo-phase ﬁeld. So, at equilibrium, the alloy must be a two-phase mixture: it mustconsist of “lumps” of (Sn) and (Pb) stuck together. More than this, the diagram tells us(Fig. 3.2b) that the (Sn) phase in our mixture contains 2% lead dissolved in it (it is 98%tin) and the (Pb) phase is 85% lead (it has 15% tin dissolved in it). And ﬁnally thediagram tells us (Fig. 3.2c) that the mixture contains 58% by weight of the (Pb) phase.To summarise, then, with the help of the phase diagram, we now know what theequilibrium constitution of our alloy is – we know:(a) the overall composition (50 wt% lead + 50 wt% tin),(b) the number of phases (two),(c) the composition of each phase (2 wt% lead, 85 wt% lead),(d) the proportion of each phase (58 wt% (Pb), 42 wt% (Sn) ).What we don’t know is how the lumps of (Sn) and (Pb) are sized or shaped. And wecan only ﬁnd that out by cutting the alloy open and looking at it with a microscope.* Now let’s try a few other alloy compositions at 170°C. Using Figs 3.2(b) and 3.2(c)you should be able to convince yourself that the following equilibrium constitutionsare consistent.(a) 25 wt% lead + 75 wt% tin,(b) two phases,(c) 2 wt% lead, 85 wt% lead,(d) 30 wt% (Pb), 70 wt% (Sn).(a) 75 wt% lead + 25 wt% tin,(b) two phases,(c) 2 wt% lead, 85 wt% lead,(d) 87 wt% (Pb), 13 wt% (Sn).(a) 85 wt% lead + 15 wt% tin,(b) one phase (just),(c) 85 wt% lead,(d) 100 wt% (Pb).(a) 95 wt% lead + 5 wt% tin,(b) one phase,(c) 95 wt% lead,(d) 100 wt% (Pb).* A whole science, called metallography, is devoted to this. The oldest method is to cut the alloy in half,polish the cut faces, etch them in acid to colour the phases differently, and look at them in the lightmicroscope. But you don’t even need a microscope to see some grains. Look at any galvanised steel ﬁre-escape or cast brass door knob and you will see the grains, etched by acid rain or the salts from people’shands.
28 Engineering Materials 2Fig. 3.2. (a) A 50–50 lead–tin alloy at 170°C has a constitution point that puts it in the (Sn) + (Pb) two-phase ﬁeld. The compositions of the (Sn) and (Pb) phases in the two-phase mixture are 2 wt% lead and85 wt% lead. Remember that, in any overall composition, or in any phase, wt% tin + wt% lead = 100%. Sothe compositions of the (Sn) and (Pb) phases could just as well have been written as 98 wt% tin and 15 wt%tin. (b) This diagram only duplicates information that is already contained in the phase diagram, but it helpsto emphasise how the compositions of the phases depend on the overall composition of the alloy. (c) The 50–50 alloy at 170°C consists of 58 wt% of the (Pb) phase and 42 wt% of the (Sn) phase. The straight-linerelations in the diagram are a simple consequence of the following requirements: (i) mass (Pb) phase + mass(Sn) phase = mass alloy; (ii) mass lead in (Pb) + mass lead in (Sn) = mass lead in alloy; (iii) mass tin in (Pb) +mass tin in (Sn) = mass tin in alloy.(a) 2 wt% lead + 98 wt% tin,(b) one phase (just),(c) 2 wt% lead,(d) 100 wt% (Sn).
Equilibrium constitution and phase diagrams 29Fig. 3.3. Diagrams showing how you can ﬁnd the equilibrium constitution of any lead–tin alloy at 200°C.Once you have had a little practice you will be able to write down constitutions directly from the phasediagram without bothering about diagrams like (b) or (c).(a) 1 wt% lead + 99 wt% tin,(b) one phase,(c) 1 wt% lead,(d) 100 wt% (Sn).For our second example, we look at alloys at 200°C. We can use exactly the samemethod, as Fig. 3.3 shows. A typical constitution at 200°C would be:(a) 50 wt% lead + 50 wt% tin,(b) two phases,
30 Engineering Materials 2(c) 45 wt% lead, 82 wt% lead,(d) 87 wt% (L), 13 wt% (Pb),and you should have no problem in writing down many others.Incompletely deﬁned constitutionsThere are places in the phase diagram where we can’t write out the full constitution. Tostart with, let’s look at pure tin. At 233°C we have single-phase liquid tin (Fig. 3.4). At231°C we have single-phase solid tin. At 232°C, the melting point of pure tin, we caneither have solid tin about to melt, or liquid tin about to solidify, or a mixture of both.If we started with solid tin about to melt we could, of course, supply latent heat ofmelting at 232°C and get some liquid tin as a result. But the phase diagram knowsnothing about external factors like this. Quite simply, the constitution of pure tin at232°C is incompletely deﬁned because we cannot write down the relative weights ofthe phases. And the same is, of course, true for pure lead at 327°C. The other place where the constitution is not fully deﬁned is where there is a horizontalline on the phase diagram. The lead–tin diagram has one line like this – it runs acrossthe diagram at 183°C and connects (Sn) of 2.5 wt% lead, L of 38.1% lead and (Pb) of81% lead. Just above 183°C an alloy of tin + 38.1% lead is single-phase liquid (Fig. 3.5).Just below 183°C it is two-phase, (Sn) + (Pb). At 183°C we have a three-phase mixture ofL + (Sn) + (Pb) but we can’t of course say from the phase diagram what the relativeweights of the three phases are.Fig. 3.4. At 232°C, the melting point of pure tin, we have a L + Sn two-phase mixture. But, without moreinformation, we can’t say what the relative weights of L and Sn are.Other phase diagramsPhase diagrams have been measured for almost any alloy system you are likely tomeet: copper–nickel, copper–zinc, gold–platinum, or even water–antifreeze. Some
Equilibrium constitution and phase diagrams 31Fig. 3.5. At 183°C we have a three-phase mixture of L + (Sn) + (Pb). Their relative weights can’t be foundfrom the phase diagram.Fig. 3.6. (a) The copper–nickel diagram is a good deal simpler than the lead–tin one, largely becausecopper and nickel are completely soluble in one another in the solid state. (b) The copper–zinc diagram ismuch more involved than the lead–tin one, largely because there are extra (intermediate) phases in betweenthe end (terminal ) phases. However, it is still an assembly of single-phase and two-phase ﬁelds.diagrams, like copper–nickel (Fig. 3.6a), are simple; others, like copper–zinc (Fig. 3.6b)are fairly involved; and a few are positively horrendous! But, as Table 3.1 shows, theonly real difference between one phase diagram and the next is one of degree. So that you know where to ﬁnd the phase diagrams you need we have listed pub-lished sources of phase diagrams in the Further Reading section. The determination ofa typical phase diagram used to provide enough work to keep a doctoral student busyfor several years. And yet the most comprehensive of the references runs to over athousand different phase diagrams!
32 Engineering Materials 2Table 3.1Feature Cu–Ni Pb–Sn Cu–Zn (Fig. 3.6a) (Fig. 3.1) (Fig. 3.6b)Melting points Two: Cu, Ni Two: Pb, Sn Two: Cu, ZnThree-phase horizontals None One: L + (Sn) + (Pb) Six: a + b + L b+g +L g +d+L g +d+ε d+e+L e+h+LSingle-phase ﬁelds Two: L, a Three: L, (Pb), (Sn) Seven: L, a, b, g, d, e, hTwo-phase ﬁelds One: L + a Three: ! L + (Pb) Twelve: ! L + a, L + b, L + γ , @ L + (Sn) @ L + d, L + e, L + h, (Sn) + (Pb) a + b, b + g, g + δ , g + e, δ + e, e + hFurther readingSources of phase diagramsM. Hansen and K. Anderko, Constitution of Binary Alloys, McGraw-Hill, 1958; and supplements, by R. P. Elliott, 1965, and F. A. Shunk, 1969.Smithells’ Metals Reference Book, 7th edition, Butterworth-Heinemann, 1992.ASM Metals Handbook, 10th edition, ASM International, 1990, Vol. 8.ProblemsDo not attempt problems 3.1 to 3.5 until you have worked through the TeachingYourself Phase Diagrams section at the end of the book.3.1 Explain brieﬂy what is meant by the following terms: (a) a eutectic reaction; (b) a eutectoid reaction.3.2 The phase diagram for the copper-antimony system is shown on the next page. The phase diagram contains the intermetallic compound marked “X” on the dia- gram. Determine the chemical formula of this compound. The atomic weights of copper and antimony are 63.54 and 121.75 respectively.
Equilibrium constitution and phase diagrams 33 1100 1000 Liquid 900 X Temperature (˚C) 800 700 600 α β 500 δ 400 ε 300 0 10 20 30 40 50 60 70 80 90 100 Cu Wt% Sb Sb Answer: Cu2Sb.3.3 The copper-antimony phase diagram contains two eutectic reactions and one eutectoid reaction. For each reaction: (a) identify the phases involved; (b) give the compositions of the phases; (c) give the temperature of the reaction. Answers: eutectic at 650°C: L(31% Sb) = α(12% Sb) + β(32% Sb). eutectic at 520°C: L(77% Sb) = Cu2Sb + δ(98% Sb). eutectoid at 420°C: β(42% Sb) = ε(38% Sb) + Cu2Sb.3.4 A copper-antimony alloy containing 95 weight% antimony is allowed to cool from 650°C to room temperature. Describe the different phase changes which take place as the alloy is cooled and make labelled sketches of the microstructure to illustrate your answer.3.5 Sketch a graph of temperature against time for a copper-antimony alloy containing 95 weight% antimony over the range 650°C to 500°C and account for the shape of your plot.
34 Engineering Materials 2Chapter 4Case studies in phase diagramsIntroductionNow for some practical examples of how phase diagrams are used. In the ﬁrst, atypical design problem, we ﬁnd out how solders are chosen for different uses. In thesecond we look at the high-technology area of microchip fabrication and study theproduction, by zone reﬁning, of ultra-pure silicon. And lastly, for some light-heartedrelief, we ﬁnd out how bubble-free ice is made for up-market cocktails.Choosing soft soldersMost soft solders are based on our old friend, the lead–tin system (Table 4.1). Softsolders are called “soft” because they are just that – soft mechanically, and soft in thesense that they melt easily. Even so, thin soldered joints can be very strong in shear.And the “thermal” softness of the solder can be a positive advantage. A good exampleof this is in the soldering of electronic components – like transistors, resistors or integ-rated circuits – into printed circuit boards. Because the components will be damagedif they get too hot, we want a solder with a low melting point. The phase diagram(Fig. 4.1) shows at a glance that the alloy we want is tin + 38% lead. Now that you arefamiliar with the Teach Yourself course you will know that the particular sort of three-phase horizontal whereTable 4.1 Properties of common soldersType Composition (wt%) Melting range (°C) Typical usesSoft; eutectic 62 Sn + 38 Pb 183 Electronic assemblies. (free-ﬂowing)Soft; general-purpose 50 Sn + 50 Pb 183–212 Joints in copper water systems; (moderately pasty) sheet metal work.Soft; plumbers’ (pasty) 35 Sn + 65 Pb 183–244 Wiped joints; car body ﬁlling.Soft; high-melting 5 Sn + 1.5 Ag 296–301 Higher temperatures. (free ﬂowing) + 93.5 PbSilver; eutectic 42 Ag + 19 Cu 610–620 High-strength; high-temperature. (free-ﬂowing) + 16 Zn + 25 CdSilver; general-purpose 38 Ag + 20 Cu 605–650 High-strength; high-temperature. (pasty) + 22 Zn + 20 Cd
Case studies in phase diagrams 35Fig. 4.1. The lead–tin phase diagram showing the compositions of the three main soft solders. The diagramtells us that, as soon as eutectic solder reaches 183°C, it melts completely and ﬂows easily into joints.Plumbers’ solder, on the other hand, has a melting range – although it starts to melt at 183°C it doesn’tbecome completely molten until it gets up to 244°C. At a middling temperature like 210°C it is a half-solid–half-liquid paste. High-melting point soft solders are nearly pure lead. They have a small melting range and,like eutectic solders, ﬂow easily into joints. Laα+βor, in our case, L a (Sn) + (Pb)is called a eutectic, from the Ancient Greek for “easy melting”. And electronic soldersare, appropriately enough, marketed under trade names like “Eutectic”. But eutecticsolders have another property. They become completely molten as soon as they areheated up past 183°C; and they ﬂow nicely into the joints, leaving small tidy ﬁllets ofsolder around each connection. You can imagine the number of faults that you couldget on a crowded circuit board if the solder did not ﬂow easily and had to be “put onwith a trowel”. There are times, however, when soft solder is – almost literally – put on with atrowel. Lead was widely used by the Romans for piping water; and it is only withinthe past ﬁfty years that copper – and more recently polymers – have replaced lead asthe major plumbing material. A vital part of the plumber’s craft was joining lengths oflead pipe together. This was done by bringing the ends of the pipes up to one anotherand gradually building a deposit of solder around the joint. The joint was “wiped” byhand with a moleskin pad as fresh solder was added, producing the very ﬁne wipedjoints shown in Fig. 4.2. Now, eutectic solder would be useless for this purpose. Itwould either be fully molten and run all over the place, or it would go solid and stickon the job in unsightly lumps. What is wanted is a pasty solder which can be graduallymoulded to the shape of the joint. Now, if we look at an alloy of tin + 65% lead on the
36 Engineering Materials 2Fig. 4.2. When we heat plumbers’ solder to about 210°C, and make it “pasty”, we can “wipe” it intoelegantly curved shapes. Lead pipes have been joined in this way for centuries.phase diagram we can see that, at around 210°C, the alloy will be a half-molten, half-solid slurry. This will work very nicely to shape without the temperature being toocritical. And there is also little chance of melting the lead pipes by accident. So this isthe sort of composition that plumbers’ solders have (Table 4.1). Actually, lead–tinalloys with a freezing range like this (called “mushy freezers” in the foundry world)are still used quite widely for things like ﬁlling-in dents in car body panels, andsoldering car radiators together. But in many cases they are used not so much becausethey are mushy freezers but because they contain less tin than eutectic solders and aretherefore cheaper. One of the interesting things about the lead–tin diagram (Fig. 4.1) is that all alloyscontaining between 2.5% and 81% of added lead start to melt at 183°C even thoughsome – as we have just seen – don’t become completely molten until they are quitea bit hotter. This is obviously a problem when we want to use soft solders in hotsurroundings, because they will rapidly lose their strength as they get near to 183°C.
Case studies in phase diagrams 37Fig. 4.3. The ﬂat plates that make up the ﬁrebox of a model steam boiler are tied together with screwedstays. To make the threads pressure-tight they must be sealed with solder.There is a nice illustration of this problem in the model traction engine that we lookedat in the ﬁrst case study in Chapter 1. If you look back you will see that the mostcritical component in the engine is the copper boiler (Fig. 1.1). The main parts of theboiler are soldered together with a “silver solder” which melts between 610 and 620°C(Table 4.1). This is an extremely strong and ductile alloy which loses little of its struc-tural strength at boiler operating temperatures. But the screwed stays that tie the ﬂatﬁrebox sides together (Figs 1.3, 4.3) present a problem. To make them pressure-tightthey need to be sealed with solder. Now, it is easy enough to silver solder the stayswhere they come out through the outside of the ﬁrebox; but it is difﬁcult to do thisinside the ﬁrebox because the gas blow torches that we normally use for silver solder-ing copper will not burn properly in a conﬁned space (an oxy-acetylene torch will, butit has a very localised ﬂame that can easily burn a hole in thin copper). Will soft solder– which of course melts much more easily than silver solder – be adequate for sealingstays inside the ﬁrebox? Model boilers typically work at a gauge pressure of 6 bar. At this pressure thetemperature of the saturated water and steam in the boiler is 159°C, only 24°C belowthe temperature at which lead–tin solders start to melt. Worse, the inner surface of theﬁrebox is hotter even than the water because it is next to the ﬁre. In fact, ordinary softsolders have been used successfully for many years inside model ﬁreboxes, probablybecause the copper is very good at conducting away the heat of the ﬁre. But there islittle room for variation – if you habitually run the boiler on hard scale-forming water,or accidentally let the water level down too far when steaming hard, or increase theboiler pressure and thus temperature to get better performance, you are likely to blowleaks big enough to put the ﬁre out. The solution is to use the high-melting point softsolder in Table 4.1 which is very close to being pure lead, and this is recommended bythe leading designers of miniature steam engines.
38 Engineering Materials 2Fig. 4.4. Stages in zone reﬁning a bar of impure silicon: (a) We start with a bar that has a uniformconcentration of impurity, C0. (b) The left-hand end of the bar is melted by a small electric tube furnace,making a liquid zone. The bar is encapsulated in a ceramic tube to stop the liquid running away. (c) Thefurnace is moved off to the right, pulling the zone with it. (d) As the zone moves, it takes in more impurityfrom the melted solid on the right than it leaves behind in the freshly frozen solid on the left. The surpluspushes up the concentration of impurity in the zone, which in turn pushes up the concentration of impurityin the next layer of solid frozen from it. (e) Eventually we reach steady state. (f) When the zone gets to theend of the bar the concentrations in both solid and liquid increase rapidly. (g) How we set up eqn. (4.1).
Case studies in phase diagrams 39Fig. 4.5. Schematic of top left corner of the “silicon-impurity” phase diagram. To make things simple, weassume that the liquidus and solidus lines are straight. The impurity concentration in the solid is then alwaysless than that in the liquid by the factor k (called the distribution coefﬁcient ).Pure silicon for microchipsThe semiconductor industry would have been impossible had not the process of zonereﬁning been invented ﬁrst. It is the standard way of producing ultrapure materials,both for research and for making silicon and germanium-based devices. Zone reﬁning works like this. We start with a bar of silicon containing a smalluniform concentration C0 of impurity (Fig. 4.4a). A small tubular electric furnace is putover the left-hand end of the bar, and this is used to melt a short length (Fig. 4.4b).Obviously, the concentration of impurity in this molten section must still be C0 as noimpurity has either left it or come into it. But before we can go any further we mustlook at the phase diagram (Fig. 4.5). To have equilibrium between the new liquid ofcomposition C0 and the existing solid in the bar, the solid must be of composition kC0.And yet the solid already has a composition of C0, (1/k) times too big. In fact, thesituation is rescued because a local equilibrium forms between liquid and solid at theinterface where they touch. The solid next to this interface loses a small amountof impurity into the liquid by diffusion, and this lowers the composition of the solid tokC0. Naturally, a gradient is produced in the composition of the solid (Fig. 4.4b), butbecause solid-state diffusion is relatively sluggish we can neglect the atomic ﬂux thatthe gradient causes in the present situation. The next stage in the zone-reﬁning process is to move the furnace slowly and stead-ily to the right. The left-hand end of the bar will then cool and refreeze but with theequilibrium composition kC0 (Fig. 4.4c). As the furnace continues to move to the rightthe freezing solid, because it contains much less impurity than the liquid, rejects thesurplus impurity into the liquid zone. This has the effect of increasing the impurityconcentration in the zone, which in turn then increases the impurity concentration inthe next layer of freshly frozen solid, and so on (Fig. 4.4d). Eventually the concentra-tions ramp themselves up to the situation shown in Fig. 4.4(e). Here, the solid ahead ofthe zone has exactly the same composition as the newly frozen solid behind the zone.This means that we have a steady state where as much impurity is removed from the
40 Engineering Materials 2zone in the form of freshly frozen solid as is taken into the zone by melting old solidahead of it; the composition of the zone itself therefore stays constant. The ﬁnal stage takes place when the furnace runs up to the end of the bar (Fig. 4.4f).The freshly frozen solid behind the zone continues to pump surplus impurity into anever-shortening zone, and the compositions of the liquid and the solid frozen from itramp themselves up again, eventually reaching in theory (but not in practice) inﬁnitevalues. Figure 4.4(f) shows what moving the molten zone along the bar has done to it: wehave removed impurity from the left-hand end of the bar and dumped it at the right-hand end; that is, we have zone reﬁned the left-hand part of the bar. Because we need to know how long the reﬁned section of the bar is, it is importantto describe the ramping up of the compositions in a quantitative way. We can do thisby writing a differential equation which describes what happens as the zone movesfrom some general position x to a new position x + δ x (Fig. 4.4g). For a bar of unitcross-section we can write the mass conservation equation (δ x)C0 − (δ x)kCL = l(δ CL ). (4.1) impurity taken impurity lost surplus impurity left in into zone by from zone in ﬁxed-volume zone which melting slice slice of freshly increases concentration of bar of frozen solid of of impurity in liquid by thickness δ x thickness δ x δ CLHere CL is the concentration of impurity in the liquid and l is the zone length. Allconcentrations are given in units of impurity atoms per unit volume. Developing eqn. (4.1) we get l(dCL ) = (C0 − kCL ) dx, (4.2)and l dCL = dx, (4.3) (C0 − kCL )which we can integrate to give l − ln (C0 − kCL ) = x + constant. (4.4) kNow the boundary condition is that, when x = 0, CL = C0 . Substituting this into eqn.(4.4) allows us to work out what the constant of integration is, and gives the solution l C − kCL − ln 0 = x. (4.5) k C0 − kC0 What we really want is the impurity concentration in the solid, CS. To get this wemanipulate eqn. (4.5) as follows. C − kCL kx ln 0 =− , (4.6) C0 − kC0 lwhich we can invert to give
Case studies in phase diagrams 41Fig. 4.6. Schematic plot of eqn. (4.9) showing how small k and long l give the best zone reﬁningperformance. kx C0 − kCL = (C0 − kC0 ) exp − . (4.7) l Substituting CS = kCL in eqn. (4.7) produces kx C0 − CS = C0 (1 − k ) exp − . (4.8) l This gives, at last, kx CS = C0 1 − (1 − k ) exp − , (4.9) l which we have plotted schematically in Fig. 4.6. Figure 4.6 is interesting because it shows that for the best reﬁning performance weneed both a long zone and an impurity that is relatively insoluble in the solid (low k).Unfortunately long liquid zones can be destabilised by convection, and impuritieswith a low k do not come to order! Commercial zone reﬁning processes may thereforeinvolve a large number of passes done one after the other (Fig. 4.7). This obviouslyadds a lot to the cost of the pure material, but the process can be speeded up consider-ably by using the multi-heater arrangement shown in Fig. 4.8.Making bubble-free icePeople who go in for expensive cocktails like to cool them with ice cubes which arecrystal clear – it adds to the aura of bejewelled, refreshing purity. Unfortunately, icecubes grown in an ordinary fridge are cloudy. So establishments which cater for up-market clients install special machines to make clear ice.
42 Engineering Materials 2Fig. 4.7. If the bar is repeatedly zone reﬁned from left to right then more and more of the impurity will beswept to the right-hand end of the bar. A large number of zone-reﬁning passes may be needed to make theleft-hand half of the bar as pure as we need. The right-hand half is cut off and recycled. Note that eqn. (4.9)can only be used to calculate the impurity distribution produced by the ﬁrst pass. A computer program has tobe written to handle each subsequent pass.Fig. 4.8. A multi-heater arrangement gives much faster zone reﬁning. The cloudiness of ordinary ice cubes is caused by thousands of tiny air bubbles. Airdissolves in water, and tap water at 10°C can – and usually does – contain 0.0030 wt%of air. In order to follow what this air does when we make an ice cube, we need to lookat the phase diagram for the H2O–air system (Fig. 4.9). As we cool our liquid solutionof water + air the ﬁrst change takes place at about −0.002°C when the composition linehits the liquidus line. At this temperature ice crystals will begin to form and, as thetemperature is lowered still further, they will grow. By the time we reach the eutecticthree-phase horizontal at −0.0024°C we will have 20 wt% ice (called primary ice) in ourtwo-phase mixture, leaving 80 wt% liquid (Fig. 4.9). This liquid will contain the max-imum possible amount of dissolved air (0.0038 wt%). As latent heat of freezing isremoved at −0.0024°C the three-phase eutectic reaction of Eutectic liquid (H2O + 0.0038 wt% air) → Eutectic mixture of (ice) + airwill take place. Finally, when all the eutectic liquid has frozen to ice, we will be leftwith a two-phase mixture of eutectic [ (ice) + air] which we can then cool down belowthe eutectic temperature of −0.0024°C. In fact, because the solubility of air in ice is sosmall (Fig. 4.9) almost all the air that was dissolved in the eutectic liquid separates outinto bubbles of air as soon as we get below the three-phase horizontal. And althoughthis air accounts for only 0.0038% by weight of the eutectic mixture, it takes up 2.92%by volume. This is why ordinary ice looks cloudy – it contains a network of air bubbleswhich scatter light very effectively.